- About this Journal ·
- Aims and Scope ·
- Article Processing Charges ·
- Articles in Press ·
- Author Guidelines ·
- Bibliographic Information ·
- Citations to this Journal ·
- Contact Information ·
- Editorial Board ·
- Editorial Workflow ·
- Free eTOC Alerts ·
- Publication Ethics ·
- Reviewers Acknowledgment ·
- Submit a Manuscript ·
- Subscription Information ·
- Table of Contents

ISRN Ceramics

Volume 2012 (2012), Article ID 428497, 17 pages

http://dx.doi.org/10.5402/2012/428497

## A Review on Infrared Spectroscopy of Borate Glasses with Effects of Different Additives

Department of Physics, University of Lucknow, Lucknow 226007, India

Received 12 July 2012; Accepted 26 August 2012

Academic Editors: Y. S. Cho, D. Jia, M. Kawashita, and C.-F. Yang

Copyright © 2012 Chandkiram Gautam et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

#### Abstract

Borate glasses are the technologically important class of glasses and play a significant role in various applications. Borate glasses contain planar BO_{3} groups as structural units, rather than tetrahedral SiO_{4} groups. The oxygen atoms are, as in SiO_{2}, again connected to two network-forming atoms, in case of boron. The radial distribution analysis describes the B_{2}O_{3} glass structure as consisting of boroxol rings, that is, planar rings containing three boron atoms and three oxygen atoms. The network forming of the B_{2}O_{3} and the SiO_{4} is affected with the addition of some metal cation additives Pb, Zn, Cd, and so forth. These additives also work as a network modifier and a nucleating agent for crystallization of glass. Therefore, the optical properties of the borate glasses have been changed significantly.

#### 1. Introduction

Glasses are supercooled liquids, transparent, and amorphous in nature. They are inorganic product of fusion which has cooled to a rigid condition without any crystallization. The main distinction between glass and crystals is the presence of long-range order in the crystal structure [1]. The optimization of such properties as a function of composition and other processing parameters requires a good knowledge of the microscopic glassy structure. For many years, glasses containing transition metal ions have attracted attention because of their potential applications in electrochemical, electronic, and electro-optic devices. A host of borate rich glasses containing alkaline earth oxides along with ZnO, PbO, TeO_{2} Bi_{2}O_{3,} MgO, CaO, SrO, and BaO as glass modifiers are optimistic materials for their probable applications in the fields of optical communications (optical fibers), laser hosts, optical filters, X- and *γ*-ray absorbers, photonic devices, and so forth [2–8]. Infrared spectroscopy (IR) is an important tool for understanding the structure and dynamics of amorphous materials. It is also used to assign the observed absorption peaks to the proper vibration of the atoms in geometric grouping. The spectra of many solids variables can affect the absorption peaks, and the assignment of vibration peaks of the atoms is very difficult. Usually, the method of repeated occurrence is followed in analysing the IR spectrum of solid materials [9, 10]. In this spectroscopy, the nature of the light matter interaction is not same as in Raman spectroscopy, and the fundamental differences of the two processes determine the selection rules, which control Raman or IR activity of normal mode of vibrations. Interaction of IR radiation with a normal mode of vibration only occurs when the electric field of radiation oscillates with same frequency as instant dipoles caused by atomic vibrations. A normal vibration is therefore, IR active only if a change in the dipole moment of the vibration occurs and is a one photon process, as only photon is absorbed [11]. Therefore, IR spectra give additional information rather than Raman spectra by which the symmetries of normal modes of vibration of molecules and crystal lattices are determined [12–15]. The spectrum of a sample is compared with the spectrum of a large number of compounds containing a common atom group or groups. Certain absorption peaks are common to certain groups and are assigned the vibration characteristics of these atom groups. Borate glasses have been the subject of numerous infrared studies because of their structural peculiarities [16–23]. A widespread set of very different borate glasses with optical, magnetic, superionic conductivity, and other technologically interesting properties are currently produced [24, 25].

#### 2. Infrared Spectroscopy

##### 2.1. Lead Borate Glasses

During the past five decades, many efforts have been taken to realize the roles of PbO in glass networks using different techniques [26–30]. PbO-B_{2}O_{3} glasses are of technological interests owing to their unique properties such as their low melting temperatures, wide glass formation regions, and good radiation shielding properties, [31–34]. IR spectra of the various PbO-B_{2}O_{3} glasses are shown in Figure 1. The nomenclature of these glasses has been listed in Table 1. IR spectra of pure B_{2}O_{3} gives two absorption band at wavenumbers 1300–1700 and 720 cm^{−1}. The absorption bands at wavenumbers range of 1300–1700 cm^{−1} are attributed to the bending vibration and stretching vibration of B–O–B in [BO_{3}] triangles [35, 36]. The addition of 10–20 mol% PbO does not affect borate network. The absorption bands below 620 cm^{−1} are attributed to vibration of PbO [37]. Therefore, PbO acts as a network participant filled in the interspaces of [BO_{3}] units in the form of Pb^{2+} ions (Figure 2(a)). The electrostatic fields of the strongly polarizing Pb^{2+} ions are affected with increase of PbO content, which might serve to increase the wavenumber of B–O–B bending vibrations [38]. Absorption band between 900 and 950 cm^{−1} was observed due to the stretching vibration of [BO_{4}] units [39]. This indicates that the addition of PbO leads to the conversion of [BO_{3}] units to [BO_{4}] units in borate glass, which is also confirmed in glass system of CeO_{2}-B_{2}O_{3} and La_{2}O_{3}-B_{2}O_{3} [39–41]. Moreover, with increase of the content of PbO from 30 to 50 mol%, the frequency of [BO_{4}] unit shifts from 945 cm^{−1} to a lower wavenumber 931 cm^{−1}. This may be due to the formation of bridging bonds of Pb–O–B (Figure 2(b)). Since the stretching force constant of Pb–O bonding is substantially lower than that of the B–O, the stretching frequency of Pb–O–B might tend to be lower. Another dominant shift in the glass (30 PbO 50 mol%) is the sharp decreasing trend from 1360 to 1315 cm^{−1}. Lorösch et al. [42] attribute the broad bond of about 1300 cm^{−1} to the vibration of B–O rings composed by [BO_{3}] and [BO_{4}] units. Therefore, the presumption that B–O rings are formed in the glasses by the connection of the bridge oxygen ions between [BO_{3}] triangles and [BO_{4}] tetrahedrons can be made (Figure 2(c)), due to the decreasing frequency of the stretching vibration of B–O–B. Subsequent additions of PbO (60–80 mol%) have the same effect on the structure of glasses. The biggest shift of 916–876 cm^{−1}, observed in PB-8 sample, indicates that when the content of PbO is up to 80 mol%, the content of Pb–O–B becomes dominant in the glass network structure. It can be presumed that the increasing polarization of Pb^{2+} with the increase content of PbO contributes to the formation of Pb^{2+}-modified boron–oxygen rings and their chains. New bands at 1016 and 1020 cm^{−1} of PB-6 and PB-7 glasses can be attributed to the absorption vibration of [BO_{4}] units [43], indicating the increasing content of [BO_{4}] units in glassy networks. The absorptions of PbO (below 620 cm^{−1}) show that PbO is one of the good network former of glasses in this region. Apart from the above discussions, it can be concluded that as PbO content exceeds 60 mol%; five bridging oxygens may be involved in glass networks: B–O–B in [BO_{3}] and [BO_{4}] units, the bridging oxygen ions between [BO_{3}] and [BO_{4}] units, Pb–O–B in bridge connection of [BO_{3}] and [BO_{4}] units, and Pb–O in covalent bonds (Figure 2(d)). Molecular dynamics represented that the radial distribution pattern is consistent with structures having a low concentration of such rings [40]. Although borate glass forms a three-dimensional network, its viscosity is substantially lower than that of silicate glass. Again, addition of alkali lowers the viscosity of the melt, but the effect is by no means as dramatic as for silicate glass [44, 45]. Introduction of alkali or moisture to alkali metal borate glasses causes some of the three-coordinate boron atoms to become four coordinate [46, 47]. The addition of various constituents in PbO-B_{2}O_{3} also affects the structural properties of these glasses.

##### 2.2. Barium Lead Borate Glasses

IR studies of BaO-PbO-B_{2}O_{3} glasses were reported by Schwarz and Ticha. In this study, it is seen that structural groups BO_{3} and BO_{4} can form borate networks [48]. These structural groups makes the complexity due to extensively overlapping bands, and they cover the spectral range from 600 cm^{−1} to 1500 cm^{−1} [56]. Figure 3 (1, 2–9) show the IR spectra of various BaO-PbO-B_{2}O_{3} glass samples. The compositional distribution of these glasses has been listed in Table 2. B–O stretching of trigonal BO_{3} units of vibrations 1200–1500 cm^{−1} and 850–1200 cm^{−1} is due to B–O stretching of tetrahedral units, while 600–800 cm^{−1} is due to bonding vibrations of B–O–B groups in various borate segments [57–59]. The IR response in the other two spectral regions changes significantly with the increase of PbO content. The intensity of two broad IR features, 850–1200 cm^{−1}, due to units decreases with increase of PbO content. Thus, PbO enters to the network as a network former. A spectral band at 806 cm^{−1} occurred due to boroxol ring formation in the glassy matrix [60].

##### 2.3. Cadmium Lead Borate Glasses

Alemi et al. give investigations of Cd-doped Pb_{2}O_{3}-B_{2}O_{3} glasses by IR spectra in the range of 400–4000 cm^{−1} and show their structures in Figure 4 [49]. In this study, the formation of boroxol ring and tetrahedral coordination inside the glassy matrix was not observed in IR spectra of these glasses, while the conversion of threefold to fourfold coordination of boron atoms in the structure of glasses was observed. The progressive substitution of boroxol rings by triborate and tetraborate groups is observed. In pure B_{2}O_{3} glass, the frequency 806 cm^{−1} is a characteristic of boroxol ring. The vanishing of 806 cm^{−1} means no boroxol ring in the glass structure. This type of behavior is also observed in B_{2}O_{3}-Li_{2}O glasses [67–69]. The IR spectra show the number of spectral bands which occurs due to various vibrational modes (symmetric triangles, tetrahedral and asymmetric units (nonbridging oxygen). A broad spectral band between the ranges from 3200 to 3600 cm^{−1} is attributed to hydroxyl or water groups [70, 71]. The structure of boron oxide glass consists of a random network of planar BO_{3} triangles with a certain fraction of six-membered (boroxol) rings (Krogh Moe’s model) [72]. These spectral bands are also seen in the borate glasses studied by Ghoneim et al. [73]. The spectral band in range from 1200 to 1600 cm^{−1} is due to the asymmetric stretching relaxation of the B–O band of trigonal BO_{3} units, while the spectral bands lies between 800 and 1200 cm^{−1}, and around 700 cm^{−1} is occurred due to the B–O bond stretching of the tetrahedral BO_{4} units and bending of B–O–B linkages, respectively. The absorption peak at 1307 cm^{−1} is the characteristic of B(III)–O–B(IV) stretching vibrations. B–O stretching vibrations of trigonal units in metaborates, pyroborates, and orthoborates are assigned at around 1357 cm^{−1} [74]. In these glasses, the boron is tetrahedrally surrounded by four oxygen atoms [75]. The band around 1292 cm^{−1} is due to B–O asymmetric stretching of BO_{3} unit. The band at 1234 cm^{−1} was found to be B–O stretching vibrations of unit in metaborate chains and orthoborates. Nonbridging oxygen in the form of BO_{4} vibrations was observed at 1005 cm^{−1} [76]. The absorption around 1000 cm^{−1} indicates the formation of diborate groups in the glassy matrix. The band at about 995 cm^{−1} is attributed to a stretching vibration of B–O–Si linkage in the glass system Na_{2}O-B_{2}O_{3}-SiO_{2}.

##### 2.4. MoO_{3}-Doped Lead Borate Glasses

The structural studies of MoO_{3}-doped Pb_{2}O_{3}-B_{2}O_{3} glasses by IR spectra show various absorption bands which are characteristics of different vibrational modes. The absorption band is at 700 cm^{−1} which indicates the presence of BO_{3} or boroxol groups in glass system containing 80% PbO and 20% B_{2}O_{3}. The absorption bands ranges from 740 to 1120 cm^{−1} and from 1130 to 1520 cm^{−1} which are attributed to the abundance of BO_{4} groups and BO_{3} groups [76, 98–101]. The presence of water in glassy matrix was confirmed by the IR study in this system, and these bands lies in the range from 3200 to 3640 cm^{−1}, which is related to the vibrations of hydrogen bonding, molecular water, BOH, or hydroxyl groups [77–79]. Thus, PbO may act as a network modifier in the same way as alkali oxide disrupting the bonds connecting neighboring SiO_{4}, BO_{3}, and BO_{4} groups. The ionic cross-links provided by lead ions (Pb^{2+}) are stronger than those provided by alkali ions. On the other hand, PbO can be incorporated into the glass as network forming Pb–O groups (PbO_{4} and PbO_{3}) [102, 103]. Pb_{2}O_{3}-B_{2}O_{3} glasses show the formation of BO_{4} groups proceeds at the rate of two tetrahedral added oxygen. This formation of tetrahedral is reduced with increasing the content of PbO above 20% because some of the lead atoms now participate in the network as PbO_{4} pyramids with the Pb atom forming the apex of the pyramid. These pyramids are assumed to preferentially bridge to BO_{3} rather than BO_{4} units [6, 104]. The change in electron distribution in the B_{3}–O bonds is at 30% of PbO, which probably results from the replacement of B_{3}–O–B_{4} by B_{3}–O–Pb bonds. The effect of the increase in the MoO_{3} content is specifically reflected first in the far-infrared spectra [105, 106].

Various glasses were synthesized in the glass system 30PbO-4MoO_{3}-(66−)B_{2}O_{3} : TiO_{2} () [50], and its detailed description was given as T_{0}: 30PbO-4MoO_{3}-66.0B_{2}O_{3}, T_{2}: 30PbO-4MoO_{3}-65.8B_{2}O_{3} : 0.2TiO_{2}, T_{4}: 30PbO-4MoO_{3}-65.6B2O3 : 0.4TiO_{2}, T_{6}: 30PbO-4MoO3-65.4B_{2}O_{3} : 0.6TiO_{2}, T_{8}: 30PbO-4MoO_{3}-65.2B_{2}O_{3} : 0.8TiO_{2}, T_{10}: 30PbO-4MoO_{3}-65.0B_{2}O_{3} : 1.0TiO_{2}, T_{15}: 30PbO-4MoO_{3}-64.5B_{2}O_{3} : 1.5TiO_{2}, T_{20}: 30PbO-4MoO_{3}-64.0B_{2}O_{3} : 2.0TiO_{2}.

The IR spectra of these glasses were recorded in the wavenumber range of 400–1600 cm^{−1} as shown in Figure 5. The absorption bands in the range lie from 1300 to 1400 cm^{−1}, 1000–1200 cm^{−1}, and another band lies at about 710 cm^{−1}. These bands were assigned due to stretching relaxations of B–O bonds of the trigonal BO_{3} units, vibrations of the BO_{4} structural units, and bending vibrations of B–O–B linkages, respectively [107]. An absorption band near 470 cm^{−1} associated with vibrations of PbO_{4} structural units in IR spectra of all the glasses. Two new bands were observed due to *υ*_{1} and *υ*_{3} vibrational modes of tetrahedral units near 890 and 836 cm^{−1} [108, 109]. The intensity of the absorption bands due to tetrahedral units was observed to decrease and the band at 890 cm^{−1} was found to be shifted slightly towards the higher frequency side, whereas the band at 836 cm^{−1} was observed and to be shifted towards lower frequency with increasing the concentration of the dopant TiO_{2} beyond 0.8 mol%. The intensity of the band associated with BO_{3} structural units was observed to increase at the expense of the band arising from BO_{4} units. The IR spectrum of glass T_{2} exhibited two additional prominent bands at 739 and 638 cm^{−1}. With increasing the concentration of TiO_{2} up to 0.8 mol%, the intensity of the band at 739 was observed to increase and shifted towards low-frequency region. With further increase in the concentration of TiO_{2}, a reversal trend in the intensity of these two bands has been observed.

##### 2.5. Zinc Lead Borate Glasses

Motke et al. [51] reported the IR study of zinc lead borate glasses in wavenumber range of 400–4000 cm^{−1 }(Figure 6). (A) 20PbO_{2}-30ZnO-50B_{2}O_{3}; (B) 25PbO_{2}-25ZnO-50B_{2}O_{3}; (C) 30PbO_{2}-20ZnO-50B_{2}O_{3}; (D) 35PbO_{2}-15ZnO-50B_{2}O_{3}; (E) 40PbO_{2}-10ZnO-50B_{2}O_{3}. This study reaches to conclusion of various vibration groups which are responsible for making their structure. An absorption band at 3450 cm^{−1} was occurred due to O–H stretching vibration [110–112]. The presence of structural units such as symmetric triangles, tetrahedral, and asymmetric units (i.e., nonbridging oxygen) were also confirmed in each glass samples, but ZnO does not affect the structure [103]. Similar vibrational studies had been also reported by Kamitsos et al., Ezz-Eldin et al., and Davis and Mott [113–115]. In these studies, it was found that the first structural group of bands lies within wavenumber range of 1200–1600 cm^{−1} which occurred due to the asymmetric stretching relaxation of the B–O band of trigonal BO_{3} units and the vibrational group from 800 to 1200 cm^{−1}. This vibrational group assigned is due to the B–O bond stretching of the tetrahedral BO_{4} units [116, 117]. The third group was observed at around 700 cm^{−1} and is due to bending of B–O–B linkages in the borate networks [118, 119]. This glass system shows the absence of boroxol ring formation. But the successive substitution of boroxol rings by triborate and tetraborate groups is observed. The pure B_{2}O_{3} glasses consist of BO_{3} and BO_{4} groups. These groups may be attached in the form of random network. This corresponds to the progressive substitution of boroxol ring by BO_{3} and BO_{4} groups [120–122]. The absorption band near 1357 cm^{−1} in 40 mol% glass was assigned to B–O stretching vibrations of trigonal units in metaborates, pyroborates, and orthoborates [123]. There was a change in the coordination number of boron with addition of boron trioxide to borate glasses. In these glasses, the boron is tetrahedrally surrounded by four oxygen atoms [124]. The band around 1292 cm^{−1} is due to B–O asymmetric stretching of BO_{3} unit [125], and bands around 1234 cm^{−1} was arisen by B–O stretching vibrations of unit in metaborate chains and orthoborates [126]. Vibrations of some boron atoms attached to nonbridging oxygen in the form of BO_{4} vibration were assigned band at 1004 cm^{−1} [36]. The formation of diborate group in present glasses had been represented by absorption around 1000 cm^{−1}. IR spectra showed the band at about 995 cm^{−1} was attributed to a stretching vibration of B–O–Si linkage [82]. The absorption band is at 993 cm^{−1} in the IR spectra; these glasses may be attributed to a stretching vibration of B–O–M (B–O–Pb) linkage, where M represents a metal ion, while band at 694 cm^{−1} was due to combined vibrations of BO_{4} and PbO_{4} groups [83–85]. The structure of the borate glasses was also affected by the different rates of cooling of the melt and quenching temperature [127]. In 40 mol% PbO content glass, the absorption at 616 cm^{−1} is due to bending of O–B–O. The lead plays dual role of Pb^{2+} cations in glass structure. First, it acts as a network modifier in the glassy matrix when these cations are ionically bonded, and secondly, if Pb–O bond is covalent, Pb^{2+} cation will act as glass former [89]. Because of this dual role, lead ions may disrupt the glass network and form BO_{4} tetrahedral. The low-frequency bands near 453 cm^{−1} in IR spectra of borate glasses can be attributed to vibration of metal cations such as Pb^{2+} or Zn^{2+} [46, 91–93].

##### 2.6. Bismuth Borate and Lead Bismuth Borate Glasses

Bobkova’s studies on bismuth borate and lead bismuth borate glasses by IR spectroscopy show extensive report that Bi_{2}O_{3} works as glass former, but still B_{2}O_{3} is required for the formation of well-transparent glasses. Figure 7 shows the IR spectra of ZnO-Bi_{2}O_{3}-B_{2}O_{3} glasses with Bi_{2}O_{3} in the wavenumber range of 450–4000 cm^{−1}. A continuous network of octahedral [BiO_{6}] groups connected through atoms of oxygen and the high polarizability of Bi^{3+} cations leads to an increase in the covalent bonding between bismuth and oxygen. IR studies of pure *γ*-B_{2}O_{3} show a broad absorption band wavenumber range of 400–550 cm^{−1}, while the adsorption bands in the range of 150–500 cm^{−1} occur due to the oscillations of the Bi–O bond. BiO_{6}, BiO_{4} and BiO_{3} are the basic structural units associated in the bismuth borate glasses, but most widely BiO_{6} group was found in these glasses [128–131].

##### 2.7. Potassium Borate Glasses

The structural information in potassium borate glasses was extensively studied by Singh et al. [53]. This study of these glass systems gives the information not only about structure, but also about the coordination number of the compound with respect to oxygen, network formers, and change in oxygen bonds of the framework which also is induced by the cations modifiers [132, 133]. IR studies of potassium borate glasses in the wavenumber range of 450–2000 cm^{−1} are shown in the Figure 8. Due to small mass as other network forming elements, the main vibrational modes associated with the glass network appear well above 500 cm^{−1} (in the mid-infrared region), and these networking modes are well separated from the metal ion site vibrational modes which are active in the far infrared region [94–96]. Boron has an ability to change its coordination number with oxygen between three and four providing a range of anionic environment that can coordinate the modifying metal ions. The main IR-absorption peaks in B_{2}O_{3} containing glasses lie at different wavenumbers of 710, 1260, and 1420 cm^{−1}. The absorption peak near 1420 cm^{−1} occurred due to the ring stretching of the boroxol groups, and the 1260 cm^{−1} vibration is due to the B–O–B bond constituting the linkage of boroxol groups to neighbouring groups [134]. The absorption bands near 680 and 1350 cm^{−1} can be attributed to bending vibrations of BO_{3} triangles and stretching vibrations of BO_{3} units with nonbridging oxygens (NBOs), respectively [135–138]. The band near 1066 cm^{−1} was observed due to B–O bond stretching vibrations from triborate, tetraborate, and pentaborate groups. This indicates that there is a formation of four-coordinated boron units with the addition of heavy metal oxide. The broad absorption peaks at around 1210 cm^{−1} can be attributed to asymmetric stretching vibrations of B–O bond in metaborates, pyroborates, and orthoborates. With the addition of fly ash, potassium borate glasses give significant change in their IR spectra. A prominent band at 950 cm^{−1} attributed to the stretching vibrations of B–O–Si linkage, as the main content of fly ash is silica. A shoulder band at 816 cm^{−1} can be assigned due to combined effect of stretching vibrations of Si–O–Si and B–O–B network [87].

##### 2.8. Lithium-Potassium Borate Glasses

IR studies of lithium-potassium borate glass system (30-)Li_{2}O-K_{2}O-10CdO-59B_{2}O_{3} (, and 30) doped with 1MnO_{2} in the wavenumber range of 400–2000 cm^{−1} show different transmission bands at different wavenumber positions (Figure 9). When glass sample was radiated with IR radiation, then portions of the incident radiation are absorbed at particular wavelengths. This characterizes the functional groups comprising the molecule and the overall configuration of the atoms as well. The IR transmission spectra of LKCBM glasses are given in Figure 9. IR spectra of these glasses show a band in the range of 400–1600 cm^{−1}. The band in the wavenumber range of 400–780 cm^{−1} was formed due to the bending vibrations of various borate arrangements, vibrations of Li cations through glass network, and deformation modes of network structures as well as vibrations of some MnO_{4} groups [36, 54, 139, 140]. The spectral band in the region 780–1100 cm^{−1} is due to the B–O asymmetric stretching of tetrahedral BO_{4} units and vibrations of diborates bridging to pentaborate groups; while the dominating transmission bands in the range of 1100–1600 cm^{−1} were assigned due to the stretching vibrations of borate units in which boron atoms are connected to the three oxygens (BO_{3} and B_{3}O_{6} units) [141, 142]. Recently, Aboud et al. reported the IR studies of these glasses in the wavenumber range of 600–2000 cm^{−1} as shown in Figure 10. The compositional distribution and assignment of IR spectra have been listed in Table 3 [55]. In this study, it was observed that the vibrational modes of the borate network are mainly active in three infrared spectral regions from 1200 to 1500 cm^{−1} (B–O stretching of trigonal units), from 800 to 1200 cm^{−1} (B–O stretching of tetrahedral units), and from 600 to 800 cm^{−1} (bending vibrations of various borate segments).

##### 2.9. Zinc and Manganese-Doped Borate Glasses

The vibration spectra of the zinc and manganese oxides containing borate glasses were obtained using KBr pellet technique in the range of 400–4000 cm^{−1}. FTIR spectrum of manganese oxides containing borate glasses is shown in Figure 11. IR spectra exhibit broad absorption bands as a consequence of the general disorder in the network, mainly due to a wide distribution of structural units occurring in these glasses. The band in low wavenumber side marked as “A” attributed to the presence of transition metal ions in bivalent state (Zn^{2+,} Mn^{2+}). The absorption bands marked as “B,” “C” and “D” are due to borate matrix. Details classifications of the appeared peaks have been presented in Table 4. The absorption peak near 700 cm^{−1} was assigned due to bending of B–O–B linkage, and peaks about at 1020 cm^{−1} were occurred due to B–O stretching of BO_{4} tetrahedra, while peaks at wavenumber 1280 cm^{−1} attributed to asymmetric stretching of B–O of trigonal BO_{3}. Absence of peak around 806 cm^{−1} indicates that borate network does not contain any boroxol ring. Generally, in pure B_{2}O_{3} glass, most of the boron is involved in B_{3}O_{6} boroxol rings [143–145]. The addition of transition metal ion breaks these rings, and increasingly BO_{3} and BO_{4} units are formed, which is reflected in Inset: magnified version of FTIR curves to prove the absence of boroxol rings our samples also [97].

##### 2.10. Lead Strontium Titanate Borosilicate Glasses

IR study of lead strontium titanate borosilicate glasses in glass system [()TiO_{3}]-[2SiO_{2}·B_{2}O_{3}]-[BaO·K_{2}O]-[La_{2}O_{3}] was studied by Srivastava [62] and Gautam et al. [63]. Five letters glass code refers to the composition of the glass. First two letters PT, 9P, and so forth designate the fraction of lead, that is, in the glass. PT refers to , that is, 100% lead (Pb) and 0% strontium. 9P, 8P, and so forth, refer to respectively. The third letter L indicates that La_{2}O_{3} is used as an additive. The last two letters 5B refer to fraction of modifier oxides BaO in the parent glass compositions. These spectra consist of broad and sharp bands in different regions of 400–4000 cm^{−1} as shown in Figures 12 and 13. The compositional changes in IR spectra are strongly influenced. These IR spectra of these glasses show ten absorption peaks. Absorption peaks in the range of 3425–3501 cm^{−1} are attributed to stretching of –OH^{−} bond inside the glassy network, and it form at nonbridging oxygen sites. Two absorption bands in the range of 1200–1750 cm^{−1} were found in all the glass samples. A single-broad absorption peak was observed in the glass lead rich glass composition, while the same peak splitted into two peaks in all Sr rich glass compositions. These spectral bands were observed due to the vibrational mode of the borate network, and these vibrational modes of the borate network are mainly due to the asymmetric stretching relaxation of the B–O bond of trigonal BO_{3} units. These vibrational modes occur at 1200–1600 cm^{−1}. The bands at around 1000 cm^{−1} are attributed to a stretching vibration of B–O–Si linkage. A broad absorption peak lies between 685 and 709 cm^{−1} and was due to the bending of B–O–B linkages in the borate glassy network [86, 146]. The low-frequency bands in the IR spectra of these glasses can be attributed to vibration of metal cation such as Pb^{2+} and was attributed to the vibrations of Pb^{2+} cations. Absorption peaks in FTIR spectra of the (Pb Sr)TiO_{3} borosilicate glasses have been listed in Table 5.

##### 2.11. Barium Strontium Titanate Borosilicate Glasses

More recently, our research group reported the IR studies of barium strontium titanate borosilicate glasses in wavenumber range of 450–4000 cm^{−1} and shown in Figure 14. The first sharp and broad absorption peak at 3440 cm^{−1} was assigned due to stretching mode of O–H bonds inside the glassy network [64]. These O–H bond groups are formed at nonbridging oxygen sites. An absorption band at wavenumber 2372 cm^{−1} (peak no. 2) was observed in the IR spectra. IR spectra show a sharp absorption at 1632 cm^{−1} (peak no. 3). A doublet absorption band occurs at wavenumbers 1351–1398 cm^{−1} (peak no. 4 a, b). The absorption peak no. 5 was observed at wavenumber 1276 cm^{−1}. These absorption bands occurred due to the vibrational mode of the borate network in borate containing glass systems and asymmetric stretching relaxation of the B–O bonds of trigonal BO_{3} units. This band lies between wavenumber range of 1200–1750 cm^{−1} [80, 81]. An absorption peak at 1025 cm^{−1} is attributed to stretching vibrations of B–O–Si linkage. Absorption band at 714 cm^{−1} occurred due to the diborate linkage of B–O–B, in the borate glassy network. In this linkage, both boron atoms are tetrahedrally coordinated with triborate superstructural units. An absorption peak at 519 cm^{−1} at low wavenumber side was also observed due to vibration of metal cation such as Ba^{2+} and Sr^{2+}.

##### 2.12. Sodium Borosilicate Glasses

IR studies of sodium borosilicate glasses show various absorption bands in the wavenumber ranges of 400–2000 cm^{−1}; it has been given in the Figures 15 and 16. The bands near 900–1100 cm^{−1} dominate over all bands. The absorption band around 970 cm^{−1} and a line near 1065 cm^{−1} were identified. Three additional weaker bands peaking near 460, 780, and 1420 cm^{−1} can be identified in the IR spectrum. When Ca and Ba are substituted for sodium, the shape of the dominant absorption band changes, and the band peak shifts into the high-frequency side [65]. In addition, the intensity of the band peaking at 1420 cm^{−1} increases, while a small bands near 715 cm^{−1} and 780 cm^{−1} shifts by approximately 20 cm^{−1} into the high-frequency region. The low-frequency sideband peaking near 460 cm^{−1} is due to deformation vibrations of the Si–O–Si bridges, and bands in the region of 780–800 cm^{−1} were formed due to deformation vibrations of the Si–O– end groupings, while the band near 970 cm^{−1} attests to the presence of BO_{4} tetrahedra in the structure of the glass [147]. The band at 1065 cm^{−1} IR spectra of the sodium glass is related with the asymmetric stretching vibrations of the Si–O–Si bonds, and the shift of its peak is due to a change of the degree of polymerization of the glass structure [148]. The absorption bands near 715 and 1420 cm^{−1} are associated with different vibrational modes of the planar BO_{3} triangles [36].

##### 2.13. Lead Bismuth Borosilicate Glasses

The IR studies of lead bismuth borate glasses had been reported by Chen et al. and shown in Figure 17. The glass compositions have been given as PBB01(50-40-10), PBB2 (40-50-10), PBB03 (20-70-10), PBB4 (35-45-20), PBB5 (15-65-20), and PBB06 (25-35-40). This absorption band occurs due to stretching mode of O–H bonds inside the glassy network. With addition of lead oxide, the band shifted towards higher wavenumber side. An absorption band between wavenumber 2867 and 2943 cm^{−1}, and it occurs due to hydrogen bonding [81]. This absorption band disappears in IR spectra when lead content increased to 40%. The vibrational mode of the borate network exhibited an absorption band between wavenumbers 1522 and 1483 cm^{−1} due to the asymmetric stretching relaxation in B–O bonds of trigonal BO_{3} units. Such types of vibrational modes occur within the wavenumbers range of 1200–1750 cm^{−1} [88]. The broad absorption band at around 1120–1153 cm^{−1} was occurred due to a stretching vibration of B–O–Si linkage [149]. IR spectra of all glass samples exhibited an absorption band within the wavenumber range of 816–833 cm^{−1} due to the diborate linkage, B–O–B, in the borate glassy network. In this linkage, both boron atoms are tetrahedrally coordinated with triborate superstructural units [150]. An absorption peaks at lower wavenumber side attributed to vibration of metal cation such as Pb^{2+} and Bi^{3+}. The assignment of various vibrations groups in IR spectra have been listed in Table 6. FTIR spectra of these glasses many absorption bands at different wavelengths region which may attributed attribute to OH-group and other borate groups. PBB01 showed more than 70% of transmittance from 2000 nm to 4000 nm. The peak around 3300 nm is due to the OH absorption. With the increase of PbO and Bi_{2}O_{3} content, the spectrum exhibits a shift to longer wavelength [66].

#### 3. Summary

In this paper, we have discussed the infrared spectroscopy of borate glasses and the effects of various additives on structural properties of these glasses. The borate glasses contain the molecular water, hydroxyl group along with hydrogen bonding which was confirmed by absorption bands in wavenumber range of 2700–3750 cm^{−1} in the IR spectra of these glasses. The amount of molecular water content affected with variation of different metallic additives. 10–20 mol% addition of PbO does not affect the borate network in lead borate glasses, while with increasing the concentration of PbO, the absorption bands below 620 cm^{−1} are attributed. Moreover, with in content from 30 to 50 mol% of PbO, bands related to the [BO_{4}] unit shifts from 945 cm^{−1} to a lower wavenumber 931 cm^{−1}. Boroxol ring formation in the glassy matrix at wavenumber 806 cm^{−1} in lead borate glasses was observed while its formation inside the glassy matrix of Cd-doped PbO-B_{2}O_{3} glasses was not observed in IR spectra. This may be lead to the conclusion that the addition of Cd in glassy matrix deformed the boroxol ring. The conversion of three-fold to four-fold coordination of boron atoms in the structure of glasses was also observed in Cd-doped PbO-B_{2}O_{3} glasses. Similarly, the presence of a stretching vibration of B–O–M (B–O–Pb) linkage, where “M” represents a metal ion in the glassy matrix of Cd, Pb, Ba, Mo, and so forth, doped borate glasses also confirmed by IR spectra and assigned near 992 cm^{−1}. The absorption band at 696 cm^{−1} is due to combined vibration of BO_{4} and PbO_{4} groups. The addition of lead in borate glass system modified the network of glassy matrix. Asymmetric stretching relaxation of B–O bonds of trigonal BO_{3} units and composite of two silicate chain and borate phases have been presented in various vibration modes such as diborate, triborate, tetraborate, orthoborate, and pyroborate in the wavenumber regions of 1200–1750 cm^{−1} and 700–1200 cm^{−1}. These networks significantly affected by additives in borate glasses. In borosilicate glasses, the addition vibrations due to presence of silica were also observed, and these vibrations present basically two forms. Firstly, the stretching vibration of B–O–Si linkages, and secondly, they may be found as stretching vibrations of Si–O–Si. The metallic cations vibrations in glassy matrix may be attributed in low wavenumber sides (<600 cm^{−1}).

#### Acknowledgments

C. R. Gautam is grateful to the University Grant Commission (UGC), New Delhi, India, for providing the financial support as a Major Research Project (File no. 37-439/2009 (SR)). C. R. Gautam and A. K. Yadav are also thankful to Uttar Pradesh Council of Science and Technology (UPCST), Lucknow, India, for providing partial financial support under “Young Scientist Scheme Research Project” (no. CSTT/YSS/D-3913). The authors also acknowledge the facilities provided by the Head Department of Physics, University of Lucknow, Lucknow 226007, India.

#### References

- M. Yamane and Y. Asahara,
*Glasses for Photonics*, Cambridge University Press, Cambridge, UK, 2000. - S. Murugavel and B. Roling, “Ion transport mechanism in borate glasses: influence of network structure on non-Arrhenius conductivity,”
*Physical Review B*, vol. 76, Article ID 180202, 4 pages, 2007. View at Publisher · View at Google Scholar - G. D. Khattak, N. Tabet, and L. E. Wenger, “Structural properties of glasses in the series (SrO)
_{x}(V_{2}O_{5})_{1−x}, (SrO)_{0.5−y}(B_{2}O_{3})_{y}(V_{2}O_{5})_{0.5}, and (SrO)_{0.2}(B_{2}O_{3})z(V_{2}O_{5})_{0.8−z},”*Physical Review B*, vol. 72, no. 10, Article ID 104203, 12 pages, 2005. View at Publisher · View at Google Scholar · View at Scopus - G. S. Murugan, E. Fargin, V. Rodriguez et al., “Temperature-assisted electrical poling of TeO
_{2}-Bi_{2}O_{3}-ZnO glasses for non-linear optical applications,”*Journal of Non-Crystalline Solids*, vol. 344, no. 3, pp. 158–166, 2004. View at Publisher · View at Google Scholar · View at Scopus - W. H. Dumbaugh and J. C. Lapp J, “Heavy-metal oxide glasses,”
*Journal of the American Ceramic Society*, vol. 75, no. 9, pp. 2315–2326, 1992. View at Publisher · View at Google Scholar - F. H. El-Batal, M. A. Azooz, and F. M. Ezz-Eldin, “Thermal expansion and infrared studies of binary Bi
_{2}O_{3}-B_{2}O_{3}and ternary Bi_{2}O_{3}-B_{2}O_{3}-PbO glasses,”*Physics and Chemistry of Glasses*, vol. 43, no. 5, pp. 260–266, 2002. View at Scopus - K. J. Rao, B. G. Rao, and S. R. Elliot, “Glass formation in the system PbO-PbCl
_{2},”*Journal of Materials Science*, vol. 20, no. 5, pp. 1678–1682, 1985. View at Publisher · View at Google Scholar - V. C. V. Gowda, R. V. Anavekar, and K. J. Rao, “Elastic properties of fast ion conducting lithium based borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 351, no. 43–45, pp. 3421–3429, 2005. View at Publisher · View at Google Scholar · View at Scopus - S. Anderson, R. L. Bohon, and I. D. Kimpton J, “Infrared spectra and atomic arrangement in fused boron oxide and soda
borate glasses,”
*Journal of the American Ceramic Society*, vol. 38, no. 10, pp. 370–377, 1955. View at Publisher · View at Google Scholar - J. Wang and C. A. Agell,
*Glass Structure By Spectroscopy*, chapter 7, Dekker, New York, NY, USA, 1976. - B. Schrader,
*Inferared and Raman Spectroscopy*, John Wiley and Sons, London, UK, 1995. - J. R. Ferraro and J. S. Jiomek,
*Introductory Group Theory and Its Applications to Molecular Structure*, Plenum Press, New York, NY, USA, 1969. - D. L. Rouseau, R. P. Bauman, and S. P. S. Porto, “Normal mode determination in crystals,”
*Journal of Raman Spectroscopy*, vol. 10, no. 1, pp. 253–290, 1981. View at Publisher · View at Google Scholar - W. G. Feteley, F. R. Dolish, N. T. McDewitt, and F. F. Bentley,
*Infered and Raman Selection Rules for Molecular and Lattice Vibrations, the Correlation Mathod*, John Wiley and Sons, London, UK, 1995. - A. M. Efimov, “Quantitative IR spectroscopy: applications to studying glass structure and properties,”
*Journal of Non-Crystalline Solids*, vol. 203, pp. 1–11, 1996. View at Publisher · View at Google Scholar · View at Scopus - D. L. Griscom,
*Borate Glasses: Structure, Properties and Applications*, Plenum, New York, NY, USA, 1978. - U. Selvaraj and K. J. Rao, “Infrared spectroscopic study of mixed-alkali effect in borate glasses,”
*Spectrochimica Acta Part A*, vol. 40, no. 11-12, pp. 1081–1085, 1984. View at Scopus - E. I. Kamitsos, M. A. Karakassides, and G. D. Chryssikos, “A vibrational study of lithium sulfate based fast ionic conducting borate glasses,”
*Journal of Physical Chemistry*, vol. 90, no. 19, pp. 4528–4533, 1986. View at Scopus - E. I. Kamitsos, M. A. Karakassides, and G. D. Chryssikos, “Cation—network interactions in binary alkali metal borate glasses. A far-infrared study,”
*Journal of Physical Chemistry*, vol. 91, no. 22, pp. 5807–5813, 1987. View at Scopus - E. I. Kamitsos, G. D. Chryssikos, A. P. Patsis, and M. A. Karakassides, “Lithium conducting borate glasses: evidence for two broad distributions of cation-hosting environments,”
*Journal of Non-Crystalline Solids*, vol. 131–133, no. 2, pp. 1092–1095, 1991. View at Scopus - U. Harder, P. Reich, and M. Willfahrt, “Infrared reflection measurements of lead Borate glasses,”
*ournal of Molecular Structure*, vol. 349, pp. 297–300, 1995. View at Publisher · View at Google Scholar - A. H. Verhoef and H. W. den Hartog, “Infrared spectroscopy of network and cation dynamics in binary and mixed alkali borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 182, no. 3, pp. 221–234, 1995. View at Scopus - A. H. Verhoef and H. W. den Hartog, “Infrared spectroscopy of network and cation dynamics in binary and mixed alkali borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 182, no. 3, pp. 221–234, 1995. View at Scopus - G. Dalba, P. Fornasini, F. Rocca, and F. Monti, “Short range order in borate glasses investigated by X-ray absorption spectroscopy,”
*Physics and Chemistry of Glasses*, vol. 41, pp. 290–295, 2000. - L. Bih, M. El Omari, J. M. Réau et al., “Electronic and ionic conductivity of glasses inside the Li
_{2}O-MoO_{3}-P_{2}O_{5}system,”*Solid State Ionics*, vol. 132, no. 1, pp. 71–85, 2000. View at Publisher · View at Google Scholar · View at Scopus - H. S. Liu, T. S. Chin, and S. W. Yung, “FTIR and XPS studies of low-melting PbO-ZnO-P
_{2}O_{5}glasses,”*Chemistry and Physics*, vol. 50, no. 1, pp. 1–10, 1997. View at Publisher · View at Google Scholar - D. Stentz, S. Blair, C. Goater, S. Feller, and M. Affatigato, “Analysis of the structure of lead borosilicate glasses using laser ionization time of flight mass spectroscopy,”
*Journal of Non-Crystalline Solids*, vol. 293-295, no. 1, pp. 416–421, 2001. View at Publisher · View at Google Scholar · View at Scopus - M. Abid, M. Et-Tabirou, and M. Taibi, “Structure and DC conductivity of lead sodium ultraphosphate glasses,”
*Materials Science and Engineering B*, vol. 97, no. 1, pp. 20–24, 2003. View at Scopus - P. J. Bray, M. Leventhal, and H. O. Hooper, “Nuclear magnetic resonance investigations of the structure of lead borate glasses,”
*Physics and Chemistry of Glasses*, vol. 4, no. 2, pp. 47–66, 1963. - B. N. Meera, A. K. Sood, N. Chandrabhas, and J. Ramakrishna, “Raman study of lead borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 126, no. 3, pp. 224–230, 1990. View at Scopus - Z. Pan, S. H. Morgan, and B. H. Long, “Raman scattering cross-section and non-linear optical response of lead borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 185, no. 1-2, pp. 127–134, 1995. View at Scopus - J. M. Wu and H. L. Huang, “Microwave properties of zinc, barium and lead borosilicate glasses,”
*Journal of Non-Crystalline Solids*, vol. 260, no. 1-2, pp. 116–124, 1999. View at Publisher · View at Google Scholar · View at Scopus - P. Srivastava, S. B. Rai, and D. K. Rai, “Effect of lead oxide on optical properties of Pr
^{3+}doped some borate based glasses,”*Journal of Alloys and Compounds*, vol. 368, no. 1-2, pp. 1–7, 2004. View at Publisher · View at Google Scholar · View at Scopus - N. Singh, K. J. Singh, K. Singh, and H. Singh, “Comparative study of lead borate and bismuth lead borate glass systems as gamma-radiation shielding materials,”
*Nuclear Instruments and Methods in Physics Research, Section B*, vol. 225, no. 3, pp. 305–309, 2004. View at Publisher · View at Google Scholar · View at Scopus - Y. Cheng, H. Xiao, W. Guo, and W. Guo, “Structure and crystallization kinetics of PbO-B
_{2}O_{3}glasses,”*Ceramics International*, vol. 33, no. 7, pp. 1341–1347, 2007. View at Publisher · View at Google Scholar · View at Scopus - E. I. Kamitsos, A. P. Patsis, M. A. Karakassides, and G. D. Chryssikos, “Infrared reflectance spectra of lithium borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 126, no. 1-2, pp. 52–67, 1990. View at Scopus - A. K. Hassan, L. Börjesson, and L. M. Torell, “The boson peak in glass formers of increasing fragility,”
*Journal of Non-Crystalline Solids*, vol. 172–174, no. 1, pp. 154–160, 1994. View at Scopus - W. L. Konijnendijk and H. Verweij, “Structural aspects of vitreous PbO
*·*2B_{2}O_{3}studied by Raman scattering,”*Journal of the American Ceramic Society*, vol. 59, no. 9-10, pp. 459–461, 1976. View at Publisher · View at Google Scholar - K. El-Egili, H. Doweidar, Y. M. Moustafa, and I. Abbas, “Structure and some physical properties of PbO-P
_{2}O_{5}glasses,”*Physica B*, vol. 339, no. 4, pp. 237–245, 2003. View at Publisher · View at Google Scholar · View at Scopus - G. El-Damrawi and K. El-Egili, “Characterization of novel CeO2-B
_{2}O_{3}glasses, structure and properties,”*Physica B*, vol. 299, no. 1-2, pp. 180–186, 2001. View at Publisher · View at Google Scholar · View at Scopus - P. J. Bray, S. A. Feller, G. E. Jellison, and Y. H. Yun, “B10 NMR studies of the structure of borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 38-39, no. 1, pp. 93–98, 1980. View at Scopus - J. Lorösch, M. Couzi, J. Pelous, R. Vacher, and A. Levasseur, “Brillouin and raman scattering study of borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 69, no. 1, pp. 1–25, 1984. View at Scopus - E. N. Boulos and N. J. Kreidl J, “Structure and properties of silver borate glasses,”
*Journal of the American Ceramic Society*, vol. 54, no. 8, pp. 368–375, 1971. View at Scopus - M. P. Teter, “Glass structure using quantum molecular dynamics,” in
*Proceedings of the 89th Annual Meeting American Ceramic Society*, p. 231, Pittsburgh, Russia, 1987. - L. Shartsis and S. Spinner, “Viscosity and density of molten optical glasses,”
*Journal of Research of the National Bureau of Standards*, vol. 46, no. 3, pp. 176–194, 1951. View at Publisher · View at Google Scholar - P. J. Bray and J. G. O'Keefe, “Nuclear magnetic resonance investigations of the structure of alkali borate glasses,”
*Physics and Chemistry of Glasses*, vol. 4, pp. 37–46, 1963. - R. Brueckner, H. U. Chun, H. Goretzki, and M. Sammet, “XPS measurements and structural aspects of silicate and phosphate
glasses,”
*Journal of Non-Crystalline Solids*, vol. 42, no. 1–3, pp. 49–60, 1980. View at Scopus - J. Schwarz and H. Ticha, “Some optical properties of BaO-PbO-B
_{2}O_{3}glasses,”*The Journal of Optoelectronics and Advanced Materials*, vol. 5, no. 1, pp. 69–74, 2003. - A. A. Alemi, H. Sedghi, A. R. Mirmohseni, and V. Golsanamlu, “Synthesis and characterization of cadmium doped lead-borate glasses,”
*Bulletin of Materials Science*, vol. 29, no. 1, pp. 55–58, 2006. View at Publisher · View at Google Scholar · View at Scopus - P. S. Prasad, M. S. Reddy, V. R. Kumar, and N. Veeraiah, “Spectroscopic and dielectric studies on PbO-MoO
_{3}-B_{2}O_{3}glasses incorporating small concentrations of TiO_{2},”*Philosophical Magazine*, vol. 87, no. 36, pp. 5763–5787, 2007. View at Publisher · View at Google Scholar · View at Scopus - S. G. Motke, S. P. Yawale, and S. S. Yawale, “Infrared spectra of zinc doped lead borate glasses,”
*Bulletin of Materials Science*, vol. 25, no. 1, pp. 75–78, 2002. View at Scopus - N. M. Bobkova, “Study of the properties of bismuth-borate systems toward low-melting lead-free glasses,”
*Glass Physics and Chemistry*, vol. 38, no. 1, pp. 180–183, 2012. View at Publisher · View at Google Scholar - J. Singh, S. P. Singh, D. Singh, G. S. Mudahar, and K. S. Thind, “Optical characterization of fly ash as a glass modifier in potassium borate glasses,”
*Materials Physics and Mechanics*, vol. 11, no. 1, pp. 17–22, 2011. View at Scopus - G. Padmaja and P. Kistaiah, “Infrared and raman spectroscopic studies on alkali borate glasses: evidence of mixed alkali effect,”
*Journal of Physical Chemistry A*, vol. 113, no. 11, pp. 2397–2404, 2009. View at Publisher · View at Google Scholar · View at Scopus - H. Aboud, H. Wagiran, I. Hossain, and R. Hussin, “Infrared spectra and energy band gap of potassium lithium borate glass
dosimetry,”
*International Journal of Physical Sciences*, vol. 7, pp. 922–926, 2012. - N. J. Kreidl,
*Inorganic Glass-Forming Systems in Glass: Science and Technology*, vol. 1 of*Glass-Forming Systems*, Academic Press, New York, NY, USA, 1983. - A. Aronne, S. Esposito, and P. Pernice, “FTIR and DTA study of structural transformations and crystallisation in BaO-B
_{2}O_{3}-TiO_{2}glasses,”*Journal of Physics and Chemistry of Glasses*, vol. 40, no. 2, pp. 63–68, 1999. View at Scopus - G. E. Jellison and P. J. Bray, “A structural interpretation of B10 and B11 NMR spectra in sodium borate glasses,”
*Journal of Non-Crystalline Solids*, vol. 29, no. 2, pp. 187–206, 1978. View at Scopus - F. L. Galeener, G. Lucovsky, and J. C. Mikkelsen Jr., “Vibrational spectra and the structure of pure vitreous B
_{2}O_{3},”*Physical Review B*, vol. 22, no. 8, pp. 3983–3990, 1980. View at Publisher · View at Google Scholar · View at Scopus - K. Shimakawa, “On the compositional dependence of the optical gap in amorphous semiconducting alloys,”
*Journal of Non-Crystalline Solids*, vol. 43, no. 2, pp. 229–244, 1981. View at Scopus - M. Pal, B. Roy, and M. Pal, “Structural characterization of borate glasses containing zinc and manganese
oxides,”
*Journal of Modern Physics*, vol. 2, pp. 1062–1066, 2011. View at Publisher · View at Google Scholar - A. K. Srivastava, “Fuzzy topology at the Banaras Hindu University, Varanasi (India),”
*Fuzzy Sets and Systems*, vol. 25, no. 3, pp. 381–382, 1988. View at Scopus - C. R. Gautam, D. Kumar, and O. Parkash, “IR study of Pb-Sr titanate borosilicate glasses,”
*Bulletin of Materials Science*, vol. 33, no. 2, pp. 145–148, 2010. View at Publisher · View at Google Scholar - A. K. Yadav and C. R. Gautam, “IR and Raman Spectroscopy of (Ba,Sr)TiO
_{3}Borosilicate Glass Doped with La_{2}O_{3},”*Lucknow Journal of Science*, vol. 8, pp. 26–30, 2011. - V. E. Eremyashev, A. A. Osipov, and L. M. Osipova, “Borosilicate glass structure with rare-earth-metal cations substituted for sodium cations,”
*Glass and Ceramics*, vol. 68, no. 7-8, pp. 205–208, 2011. View at Publisher · View at Google Scholar - Q. Chen, Q. Chen, and S. Wang, “A new Faraday rotation measurement method for the study on magneto
optical property of PbO-Bi
_{2}O_{3}-B_{2}O_{3}glasses for current sensor applications,”*Open Journal of Inorganic Non-metallic Materials*, vol. 1, pp. 1–7, 2011. View at Publisher · View at Google Scholar - K. El-Egili and A. H. Oraby, “The structure and electrical properties of lithium borate glasses containing thallic oxide,”
*Journal of Physics Condensed Matter*, vol. 8, no. 46, pp. 8959–8970, 1996. View at Publisher · View at Google Scholar · View at Scopus - A. R. Kulkarni, H. S. Maiti, and A. Paul, “Fast ion conducting lithium glasses—review,”
*Bulletin of Materials Science*, vol. 6, no. 2, pp. 201–221, 1984. View at Publisher · View at Google Scholar - M. A. Kanehisa and R. J. Elliot, “Vibrations of boron oxide glass,”
*Materials Science and Engineering B*, vol. 3, no. 1-2, pp. 163–166, 1989. View at Publisher · View at Google Scholar - R. V. Adams and R. W. Douglas, “Infra-red studies on various samples of fused silica with special reference to the bands due to water,”
*Journal of The Society of Glass Technology*, vol. 43, pp. 147–158, 1959. - H. Scholzelt,
*Glass: Nature, Structure and Properties*, Springer, New York, NY, USA, 1991. - J. Krogh-Moe, “Interpretation of the infra-red spectra of boron oxide and alkali borate glasses,”
*Physics and Chemistry of Glasses*, vol. 6, pp. 46–54, 1965. - N. A. Ghoneim, H. A. El Batal, N. Abdel Shafi, and M. H. Azooz, “Synthesis and Characterization of Cadmium Doped Lead-Borate Glasses,” in
*Proceeding of the Egyptian Conference of Chemistry*, p. 162, Cairo, Egypt, 1996. - V. G. Chekhovskii, “The Interpretation of IR Spectra of Alkali Borate Glasses,”
*Fizika i Khimiya Stekla*, vol. 11, p. 24. - H. M. Heaton and H. Moore,
*Journal Physics and Chemistry of Glasses*, vol. 28, p. 203, 1987. - J. Biscoe and B. E. Warren, “X-ray diffraction study of soda-boric oxide glass,”
*Journal of the American Ceramic Society*, vol. 21, no. 8, pp. 287–293, 1938. View at Publisher · View at Google Scholar - M. F. Mydlar, N. J. Kreidl, and J. K. Hendren, “X-ray diffraction study of lead silicate glasses,”
*Physics and Chemistry of Glasses*, vol. 11, p. 198, 1970. - U. Selveraj and K. J. Rao, “Role of lead in lead phosphomolybdate glasses and a model of structural units,”
*Journal of Non-Crystalline Solids*, vol. 104, no. 2-3, pp. 300–315, 1988. View at Publisher · View at Google Scholar - A. Varshneya,
*Fundamentals of Inorganic Glasses*, Academic Press, New York, NY, USA, 1994. - A. Venktaraman, V. A. Hiremath, S. K. Date, and S. D. Kulkarni, “A new combustion route to
*γ*-Fe_{2}O_{3}synthesis,”*Bulletin of Materials Science*, vol. 24, no. 6, pp. 617–621, 2001. View at Publisher · View at Google Scholar - G. Sharma, K. Singh, Manupriya, S. Mohan, H. Singh, and S. Bindra, “Effects of gamma irradiation on optical and structural properties of PbO-Bi
_{2}O_{3}-B_{2}O_{3}glasses,”*Radiation Physics and Chemistry*, vol. 75, no. 9, pp. 959–966, 2006. View at Publisher · View at Google Scholar · View at Scopus - T. F. Soules, “A molecular dynamic calculation of the structure of B
_{2}O_{3}glass,”*The Journal of Chemical Physics*, vol. 73, no. 8, pp. 4032–4036, 1980. View at Scopus - K. Nakamoto,
*Infrared & Raman Spectra of Inorganic & Coordination Compounds*, John Wiley, New York, NY, USA, 4th edition, 1992. - A. S. Tenny and J. Wong, “Vibrational spectra of vapor-deposited binary borosilicate glasses,”
*Journal of Chemical Physics*, vol. 56, pp. 5516–5523, 1972. View at Publisher · View at Google Scholar - H. M. Heaton and H. Moore, “The sources of the infra-red absorption bands observed in the trans-mission curves of the glasses,”
*Journal of the Society of Glass Technology*, vol. 41, p. 28, 1957. - C. Gejke, E. Zanghellini, J. Swenson, and L. Börjesson, “Microscopic structure of tin-borate and tin-boratephosphate glasses,”
*Journal of Power Sources*, vol. 119-121, pp. 576–580, 2003. View at Publisher · View at Google Scholar · View at Scopus - I. Waclawska, “Glass transition effect of amorphous borates,”
*Thermochimica Acta*, vol. 269, pp. 457–464, 1995. View at Publisher · View at Google Scholar - R. C. lucacel and I. Ardelean, “Comparative structural investigation of B
_{2}O_{3}-MO-CuO glasses (MO → TeO_{2}or As_{2}O_{3}) by FTIR and Raman spectroscopies,”*Journal of Optoelectronics and Advanced Materials*, vol. 8, pp. 1124–1128, 2006. - A. M. Azhra and C. Y. Zahra, “DSC and Raman studies of lead borate and lead silicate glasses,”
*Journal of Non-Crystalline Solids*, vol. 155, pp. 45–55, 1993. View at Publisher · View at Google Scholar - P. G. Bray and J. G. O'Keefe, “Nuclear magnetic resonance investigations of the structure of alkali borate glasses,”
*Physics and Chemistry of Glasses*, vol. 4, pp. 37–46, 1963. - H. Doweidar, M. A. A. Zeid, and G. M. El-Damrawy, “Effect of gamma radiation and thermal treatment on some physical properties of ZnO-PbO-B
_{2}O_{3}glasses,”*Journal of Physics D*, vol. 24, no. 12, pp. 2222–2228, 1991. View at Publisher · View at Google Scholar · View at Scopus - S. P. Yawale, S. V. Pakade, and C. S. Adgaonkar, “Infrared spectra of some borate glasses,”
*Indian Journal of Pure and Applied Physics*, vol. 33, pp. 34–37, 1995. - S. A. Feller, N. Lower, and M. Affatigato, “Density as a probe of oxide glass structure,”
*Physics and Chemistry of Glasses*, vol. 42, no. 3, pp. 240–246, 2001. View at Scopus - E. I. Kamitsos, “Infrared studies of borate glasses,”
*Physics and Chemistry of Glasses*, vol. 44, no. 2, pp. 79–87, 2003. View at Scopus - A. Karki, S. Feller, H. P. Lim, J. Stark, C. Sanchez, and M. Shibata, “The density of sodium-borate glasses related to atomic arrangements,”
*Journal of Non-Crystalline Solids*, vol. 92, no. 1, pp. 11–19, 1987. View at Scopus - H. P. Lim and S. Feller, “The density of low metal content rubidium, cesium, silver, and thallium borate glasses related to atomic arrangements,”
*Journal of Non-Crystalline Solids*, vol. 94, no. 1, pp. 36–44, 1987. View at Scopus - W. Soppe, J. Kleerebezem, and H. W. D. Hartog, “Raman spectroscopy study of (B
_{2}O_{3})_{1−x−y}(Li_{2}O)_{x}(Li_{2}Cl_{2})_{y}and (B_{2}O_{3})_{1−x−y}(Li_{2}O)_{x}(Cs_{2}O)_{y},”*Journal of Non-Crystalline Solids*, vol. 93, no. 1, pp. 142–154, 1987. View at Scopus - Y. Ito and K. Miyauchi, “Ionic conductivity of Li
_{2}OB_{2}O_{3}thin films,”*Journal of Non-Crystalline Solids*, vol. 57, no. 3, pp. 389–400, 1983. View at Scopus - A. Abou Shama and F. H. El-Batal, “Structural analysis of glassy lead borate containing MoO
_{3}in relation to its optical properties,”*Egyptian Journal of Solids*, vol. 29, no. 1, pp. 49–67, 2006. - G. El-Deen and A. E.-R. Yahya, “Studies on some lithium- borate glasses containing iron and copper,”
*Turkish Journal Of Physics*, vol. 27, pp. 255–262, 2003. - A. Moguš-Milanković, A. Šantić, A. Gajović, and D. E. Day, “Spectroscopic investigation of MoO
_{3}-Fe_{2}O_{3}-P_{2}O_{5}and SrO-Fe_{2}O_{3}-P_{2}O_{5}glasses. Part I,”*Journal of Non-Crystalline Solids*, vol. 325, no. 1–3, pp. 76–84, 2003. View at Publisher · View at Google Scholar · View at Scopus - T. Hubert, U. Harder, G. Mosel, and K. Witke, “Structural investigations of lead and strontium borate glasses,” in
*Proceedings of the 2nd International Conference on Borates Glasses, Crystals and Melts*, A. C. Wright, S. A. Feller, and A. C. Hannon, Eds., pp. 156–163, Society of Glass Technology, Sheffield, UK, 1997. - P. Znášik and M. Jamnický, “Preparation, infrared spectra and structure of glasses in the system CuCl-Cu
_{2}O-(P_{2}O_{5}+ MoO_{3}),”*Journal of Non-Crystalline Solids*, vol. 146, no. C, pp. 74–80, 1992. View at Scopus - C. P. Varsamis, E. I. Kamitsos, N. Machida, and T. Minami, “Coordination states of molybdenum and the nature of copper ion sites in the superionic glasses xCuI
*·*(1 - X)Cu_{2}MoO_{2}(x = 0.4, 0.5) studied by infrared reflectance spectroscopy,”*Journal of Physical Chemistry B*, vol. 101, no. 19, pp. 3734–3741, 1997. View at Scopus - A. A. El-Kheshen, F. H. El-Batal, and S. Y. Marzouk, “UV-visible, infrared and Raman spectroscopic and thermal studies of tungsten doped lead borate glasses and the effect of ionizing gamma irradiation,”
*Indian Journal of Pure and Applied Physics*, vol. 46, no. 4, pp. 225–238, 2008. View at Scopus - M. Leventhal and P. J. Bray, “Nuclear magnetic resonance investigations of compounds and glasses in the systems PbO-B
_{2}O_{3}and PbO-SiO_{2},”*Physics and Chemistry of Glasses*, vol. 6, pp. 113–125, 1966. - A. A. Ahmed, N. Abd Elshafi, and M. R. Eltohamy,
*Indian Journal of Pure and Applied Physics*, vol. 36, p. 335, 1998. - G. Govindaraj, N. Baskaran, K. Shahi, and P. Monoravi, “Preparation, conductivity, complex permittivity and electric modulus in AgIAg
_{2}OSeO_{3}MoO_{3}glasses,”*Solid State Ionics*, vol. 76, no. 1-2, pp. 47–55, 1995. View at Scopus - N. Machida and H. Eckert, “FT-IR, FT-Raman and 95Mo MAS-NMR studies on the structure of ionically conducting glasses in the system AgI-Ag
_{2}O-MoO_{3},”*Solid State Ionics*, vol. 107, no. 3-4, pp. 255–268, 1998. View at Scopus - P. G. Bray,
*Interaction of Radiation with Solids*, Plenum, New York, NY, USA, 1967. - H. Dunken and R. H. Doremus, “Short time reactions of a Na
_{2}O-CaO-SiO_{2}glass with water and salt solutions,”*Journal of Non-Crystalline Solids*, vol. 92, no. 1, pp. 61–72, 1987. View at Scopus - R. D. Husung and R. H. Doremus, “Infrared transmission spectra of four silicate glasses before and after exposure to water,”
*Journal of Materials Research*, vol. 5, no. 10, pp. 2209–2217, 1990. View at Scopus - E. I. Kamitsos, M. A. Karakassides, and G. D. Chryssikos, “Vibrational spectra of magnesium-sodium-borate glasses. 2. Raman and mid-infrared investigation of the network structure,”
*Journal of Physical Chemistry*, vol. 91, no. 5, pp. 1073–1079, 1987. View at Scopus - F. M. Ezz-Eldin, N. A. E. L. Alaily, F. A. Khalifa, and H. A. E. L. Batal, “Fundamental of glass science and technology,” in
*Proceedings of the 3rd ESG Conference*, Verlag Der Deutschen Glastechnischen Gesellschaft, Germany, 1995. - E. A. Davis and N. F. Mott, “Conduction in non-crystalline systems V,”
*Philosophical Magazine*, vol. 22, no. 179, pp. 903–922, 1970. View at Scopus - H. B. George, C. Vira, C. Stehle et al., “A structural analysis of the physical properties of bismuth and lead based glasses,”
*Physics and Chemistry of Glasses*, vol. 40, no. 6, pp. 326–332, 1999. View at Scopus - V. R. Kumar, N. Veeraiah, S. Buddhudu, and V. J. T. Raju, “Dielectric dispersion in CuO doped ZnF
_{2}-PbO-TeO_{2}glasses,”*Journal de Physique III*, vol. 7, no. 5, pp. 951–961, 1997. View at Publisher · View at Google Scholar - I. N. Chakraborty and D. E. Day, “Effect of R
^{3+}ions on the structure and properties of lanthanum borate glasses,”*Journal of the American Ceramic Society*, vol. 68, no. 12, pp. 641–645, 1985. View at Scopus - J. C. Lapp and J. E. Shelby, “Structure-property relations in lanthanide borate glasses,”
*Journal of the American Ceramic Society*, vol. 68, no. 7, pp. 368–371, 1985. View at Scopus - V. Dimitrov, Y. Dimitriev, and A. Montenero, “IR spectra and structure of V
_{2}O_{5}GeO_{2}Bi_{2}O_{3}glasses,”*Journal of Non-Crystalline Solids*, vol. 180, no. 1, pp. 51–57, 1994. View at Scopus - R. Lal and N. D. Sharma, “Infrared spectroscopic study of zinc doped iron borate glasses,”
*Indian Journal of Pure and Applied Physics*, vol. 43, no. 11, pp. 828–832, 2005. View at Scopus - R. Lal, N. D. Sharma, H. K. Sharma, and K. Chandra, “Mössbauer and infrared studies of manganese doped iron borate glasses,”
*Indian Journal of Pure and Applied Physics*, vol. 42, no. 1, pp. 25–30, 2004. View at Scopus - R. Lal, N. D. Sharma, and K. Chandra, “Mössbauer and infrared studies of some glasses and glass-ceramics from the
*X*MnO(40−*X*)YFe_{2}O_{3}.10Al_{2}O_{3}.50B_{2}O_{3}system,”*Indian Journal of Pure and Applied Physics*, vol. 42, no. 7, pp. 498–505, 2004. View at Scopus - M. B. Saisudha and J. Ramakrishna, “Optical absorption of Nd
^{3+}, Sm^{3+}and Dy^{3+}in bismuth borate glasses with large radiative transition probabilities,”*Optical Materials*, vol. 18, no. 4, pp. 403–417, 2002. View at Publisher · View at Google Scholar · View at Scopus - H. B. Pan, X. L. Zhao, X. Zhang et al., “Strontium borate glass: potential biomaterial for bone regeneration,”
*Journal of the Royal Society Interface*, vol. 7, no. 48, pp. 1025–1031, 2010. View at Publisher · View at Google Scholar · View at Scopus - H. A. El-Batal, F. A. Khalifa, and M. A. Azooz, “Gamma ray interaction, crystallization and infrared absorption spectra of some glasses and glass-ceramics from the system Li
_{2}O.B_{2}O_{3}.Al_{2}O_{3},”*Indian Journal of Pure and Applied Physics*, vol. 39, no. 9, pp. 565–573, 2001. View at Scopus - W. Soppe, C. van der Marel, W. F. van Gunsteren, and H. W. den Hartog, “New insights into the structure of B
_{2}O_{3}glass,”*Journal of Non-Crystalline Solids*, vol. 103, no. 2-3, pp. 201–209, 1988. View at Scopus - A. V. Egorysheva, V. I. Burkov, Y. F. Kargin, V. G. Plotnichenko, and V. V. Koltashev, “Vibrational spectra of crystals of bismuth borates,”
*Crystallography Reports*, vol. 50, no. 1, pp. 127–136, 2005. View at Publisher · View at Google Scholar · View at Scopus - N. Atsusni, “Optisches Glas,” Patent no. 102007050172, Germany, 2008.
- W. Qiao and P. Chena, “Study on the properties of Bi
_{2}O_{3}-B_{2}O_{3}-BaO lead-free glass using in the electronic pastes,”*Glass Physics and Chemistry*, vol. 36, no. 3, pp. 304–308, 2010. View at Publisher · View at Google Scholar · View at Scopus - C. Yin, X. Hanning, and G. Wenning, “Influences of La
^{3+}and Er^{3+}on structure and properties of Bi_{2}O_{3}-B_{2}O_{3}glass,”*Ceramics International*, vol. 34, no. 5, pp. 1335–1339, 2008. View at Publisher · View at Google Scholar - L. Stoch and M. Sroda, “Infrared spectroscopy in the investigation of oxide glasses structure,”
*Journal of Molecular Structure*, vol. 511-512, pp. 77–84, 1999. View at Publisher · View at Google Scholar - A. Pan and A. Ghosh, “New family of lead-bismuthate glass with a large transmitting window,”
*Journal of Non-Crystalline Solids*, vol. 271, no. 1, pp. 157–161, 2000. View at Publisher · View at Google Scholar · View at Scopus - H. P. Lim, A. Karki, S. Feller, J. E. Kasper, and G. Sumcad, “The density of potassium borate glasses related to atomic arrangements,”
*Journal of Non-Crystalline Solids*, vol. 91, no. 3, pp. 324–332, 1987. View at Scopus - R. D. Shannon, “Revised effective ionic radii and systematic studies of interatomic distances in halides and chalcogenides,”
*Acta Crystallographica A*, vol. 32, pp. 751–767, 1976. View at Publisher · View at Google Scholar - J. Krogh-Moe, “The crystal structure of silver tetraborate Ag
_{2}O.4B_{2}O_{3},”*Acta Crystallographica*, vol. 189, pp. 77–81, 1965. View at Publisher · View at Google Scholar - I. Ardelean and M. Toderaş, “FTIR structural investigation of 3B
_{2}O_{3}-BaO glass matrix containing manganese ions,”*Journal of Optoelectronics and Advanced Materials*, vol. 8, no. 3, pp. 1118–1120, 2006. View at Scopus - S. Bale and S. Rahman, “Spectroscopic and physical properties of ${\text{Bi}}_{\text{2}}{\text{O}}_{\text{3}}$-${\text{B}}_{\text{2}}{\text{O}}_{\text{3}}$-ZnO-${\text{Li}}_{\text{2}}\text{O}$ glasses,”
*ISRN Spectroscopy*, vol. 2012, Article ID 634571, 7 pages, 2012. View at Publisher · View at Google Scholar - R. A. Condrate, “Vibrational spectra of structural units in glass,”
*Journal of Non-Crystalline Solids*, vol. 84, no. 1–3, pp. 26–33, 1986. View at Scopus - Y. Tetsuji, K. Noboru, S. Shuichi, and Y. Masayuki, “Structural investigation of sodium borate glasses and melts by Raman spectroscopy. II. Conversion between BO
_{4}and BO_{2}O- units at high temperature,”*Journal of Non-Crystalline Solids*, vol. 321, no. 3, pp. 147–156, 2003. View at Publisher · View at Google Scholar · View at Scopus - J. A. Duffy and M. D. Ingram, “Optical basicity-IV: influence of electronegativity on the Lewis basicity and solvent properties of molten oxyanion salts and glasses,”
*Journal of Inorganic and Nuclear Chemistry*, vol. 37, pp. 1203–1206, 1975. View at Publisher · View at Google Scholar - A. Ryichi, O. Norikazu, and U. Norimasa, “Raman spectra of K
_{2}O-B_{2}O_{3}glasses and melts,”*Journal of Non-Crystalline Solids*, vol. 293, pp. 471–476, 2001. View at Publisher · View at Google Scholar - A. H. Verhoef and H. W. den Hartog, “A molecular dynamics study of B
_{2}O_{3}glass using different interaction potentials,”*Journal of Non-Crystalline Solids*, vol. 146, no. C, pp. 267–278, 1992. View at Scopus - S. Ram, “Infrared study of the dynamics of boroxol rings in the crystallization of BaFe
_{12}O_{19}microcrystals in borate glasses,”*Physical Review B*, vol. 51, no. 10, pp. 6280–6286, 1995. View at Publisher · View at Google Scholar · View at Scopus - N. M. Bobkova and S. A. Khot'ko, “Zinc oxide in borate glass-forming systems,”
*Glass and Ceramics*, vol. 62, no. 5-6, pp. 167–170, 2005. View at Publisher · View at Google Scholar - E. I. Kamitsos and M. A. Karakassides, “Structural studies of binary and pseudo binary sodium borate glasses of high sodium content,”
*Physics and Chemistry of Glasses*, vol. 30, no. 1, pp. 19–26, 1989. View at Scopus - K. El-Egili, “Infrared studies of Na
_{2}O-B_{2}O_{3}-SiO_{2}and Al_{2}O_{3}-Na_{2}O-B_{2}O_{3}-SiO_{2}glasses,”*Physica B*, vol. 325, pp. 340–348, 2003. View at Publisher · View at Google Scholar · View at Scopus - J. Wan, J. Cheng, and P. Lu, “The coordination state of B and Al of borosilicate glass by IR spectra,”
*Journal of Wuhan University of Technology*, vol. 23, no. 3, pp. 419–421, 2008. View at Publisher · View at Google Scholar - A. S. Tenny and J. J. Wong, “Vibrational spectra of vapor-deposited binary borosilicate glasses,”
*Chemical Physics*, vol. 56, pp. 5516–5523, 1972. - R. N. Sinclair, C. E. Stone, A. C. Wright et al., “Inelastic neutron scattering studies of superstructural units in borate glasses and crystalline phases,”
*Physics and Chemistry of Glasses*, vol. 41, no. 5, pp. 286–289, 2000. View at Scopus